# Electronic Supplementary Material (ESI) for RSC Advances.
# This journal is © The Royal Society of Chemistry 2016

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_shelx
_database_code_depnum_ccdc_archive 'CCDC 1494913'
_audit_update_record             
;
2016-07-20 deposited with the CCDC.
2016-10-28 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/7
_shelx_SHELXL_version_number     2014/7
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C16 H16 Ag10 Mo12 N24 O44 P'
_chemical_formula_sum            'C16 H16 Ag10 Mo12 N24 O44 P'
_chemical_formula_weight         3509.48

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   11.0695(4)
_cell_length_b                   12.3229(5)
_cell_length_c                   13.1699(5)
_cell_angle_alpha                79.160(3)
_cell_angle_beta                 66.215(3)
_cell_angle_gamma                72.255(3)
_cell_volume                     1561.31(11)
_cell_formula_units_Z            1
_cell_measurement_temperature    298(2)
_cell_measurement_reflns_used    20476
_cell_measurement_theta_min      3.303
_cell_measurement_theta_max      29.312

_exptl_crystal_description       block
_exptl_crystal_colour            red
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.733
_exptl_crystal_F_000             1621
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          ?
_exptl_crystal_size_mid          ?
_exptl_crystal_size_min          ?
_exptl_absorpt_coefficient_mu    5.515
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      298(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   'fine-focus sealed tube'
_diffrn_measurement_device_type  'multiwire proportional'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            20476
_diffrn_reflns_av_unetI/netI     0.0427
_diffrn_reflns_av_R_equivalents  0.0307
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_theta_min         3.303
_diffrn_reflns_theta_max         29.312
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.867
_diffrn_measured_fraction_theta_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.867
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.867
_diffrn_reflns_point_group_measured_fraction_full 0.998
_reflns_number_total             8536
_reflns_number_gt                6088
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker FRAMBO'
_computing_cell_refinement       'Bruker FRAMBO'
_computing_data_reduction        'Bruker SHELXTL'
_computing_structure_solution    'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0241P)²+30.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_number_reflns         7404
_refine_ls_number_parameters     482
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0653
_refine_ls_R_factor_gt           0.0493
_refine_ls_wR_factor_ref         0.1036
_refine_ls_wR_factor_gt          0.0974
_refine_ls_goodness_of_fit_ref   1.044
_refine_ls_restrained_S_all      1.044
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
C1 C 0.8683(11) 0.1011(9) 0.3487(9) 0.037(2) Uani 1 1 d . . . . .
H1 H 0.9523 0.1029 0.2924 0.044 Uiso 1 1 calc R U . . .
C2 C 0.6979(12) 0.1276(10) 0.5015(10) 0.046(3) Uani 1 1 d . . . . .
H2 H 0.6392 0.1509 0.5719 0.055 Uiso 1 1 calc R U . . .
C3 C 0.9205(9) -0.2663(7) 0.0962(7) 0.0204(17) Uani 1 1 d . . . . .
H3 H 0.9548 -0.3006 0.1516 0.024 Uiso 1 1 calc R U . . .
C4 C 0.8649(11) -0.2406(7) -0.0444(8) 0.034(2) Uani 1 1 d . . . . .
H4 H 0.8538 -0.2536 -0.1070 0.041 Uiso 1 1 calc R U . . .
C5 C 0.5642(9) -0.2508(7) 0.1880(8) 0.0234(18) Uani 1 1 d . . . . .
H5 H 0.6165 -0.2700 0.2321 0.028 Uiso 1 1 calc R U . . .
C6 C 0.4730(11) -0.2609(8) 0.0798(9) 0.035(2) Uani 1 1 d . . . . .
H6 H 0.4475 -0.2891 0.0329 0.042 Uiso 1 1 calc R U . . .
C7 C 0.5539(9) 0.2529(7) 0.2125(9) 0.028(2) Uani 1 1 d . . . . .
H7 H 0.4747 0.2800 0.2723 0.034 Uiso 1 1 calc R U . . .
C8 C 0.7380(10) 0.2431(8) 0.0778(9) 0.033(2) Uani 1 1 d . . . . .
H8 H 0.8151 0.2622 0.0231 0.040 Uiso 1 1 calc R U . . .
N1 N 0.8210(9) 0.1480(8) 0.4447(8) 0.040(2) Uani 1 1 d . . . . .
N2 N 0.7826(7) 0.0525(6) 0.3435(7) 0.0259(17) Uani 1 1 d . . . . .
N3 N 0.6740(8) 0.0692(8) 0.4410(8) 0.038(2) Uani 1 1 d . . . . .
N5 N 0.8272(9) -0.1388(6) -0.0065(6) 0.0295(18) Uani 1 1 d . . . . .
N6 N 0.8654(8) -0.1562(6) 0.0842(6) 0.0254(16) Uani 1 1 d . . . . .
N7 N 0.9210(9) -0.3231(6) 0.0175(6) 0.0281(18) Uani 1 1 d . . . . .
N8 N 0.4895(8) -0.1472(6) 0.1756(6) 0.0242(16) Uani 1 1 d . . . . .
N9 N 0.4299(8) -0.1531(6) 0.1030(7) 0.0278(17) Uani 1 1 d . . . . .
N10 N 0.5896(8) 0.1507(6) 0.1776(7) 0.0265(17) Uani 1 1 d . . . . .
N11 N 0.7124(8) 0.1430(7) 0.0882(7) 0.0322(19) Uani 1 1 d . . . . .
N12 N 0.6441(7) 0.3137(6) 0.1523(7) 0.0248(16) Uani 1 1 d . . . . .
N13 N 0.5570(7) 0.6741(6) 0.1302(6) 0.0236(16) Uiso 1 1 d . . . . .
O21 O 1.2477(11) -0.4126(6) 0.5620(7) 0.079(4) Uani 1 1 d . . . . .
O22 O 1.3600(11) -0.6103(6) 0.4686(7) 0.074(4) Uani 1 1 d . . . . .
01 O 1.4831(6) -0.4333(6) 0.3755(6) 0.0298(15) Uani 1 1 d . . . . .
02 O 1.2268(9) -0.3056(7) 0.3775(8) 0.063(3) Uani 1 1 d . . . . .
03 O 1.0021(7) -0.7012(7) 0.3258(7) 0.047(2) Uani 1 1 d . . . . .
04 O 1.2418(8) -0.6649(6) 0.2616(8) 0.053(2) Uani 1 1 d . . . . .
05 O 0.6233(6) -0.1918(6) 0.3873(5) 0.0306(15) Uani 1 1 d . . . . .
06 O 1.1457(9) -0.3471(7) 0.2283(9) 0.064(3) Uani 1 1 d . . . . .
07 O 1.0503(7) -0.5102(6) 0.2072(7) 0.045(2) Uani 1 1 d . . . . .
08 O 1.2686(7) -0.7718(9) 0.4477(5) 0.055(3) Uani 1 1 d . . . . .
09 O 1.1012(8) -0.1233(6) 0.2663(6) 0.0396(18) Uani 1 1 d . . . . .
010 O 0.8955(7) -0.2368(9) 0.3440(6) 0.052(2) Uani 1 1 d . . . . .
011 O 1.0210(7) -0.8055(9) 0.5118(6) 0.052(2) Uani 1 1 d . . . . .
012 O 0.8397(7) -0.5864(6) 0.2106(6) 0.0360(16) Uani 1 1 d . . . . .
013 O 1.3186(8) -0.5113(7) 0.0833(6) 0.048(2) Uani 1 1 d . . . . .
014 O 1.3350(9) -0.5011(6) 0.2833(8) 0.061(3) Uani 1 1 d . . . . .
015 O 1.2245(7) -0.8887(6) 0.3144(8) 0.050(2) Uani 1 1 d . . . . .
016 O 0.9411(10) -0.3721(9) 0.4843(9) 0.071(3) Uani 1 1 d . . . . .
017 O 1.0478(11) -0.5590(9) 0.3953(9) 0.072(3) Uani 1 1 d . . . . .
018 O 1.1074(11) -0.4474(9) 0.4023(9) 0.077(3) Uani 1 1 d . . . . .
019 O 0.8737(11) -0.4819(10) 0.4635(9) 0.075(3) Uani 1 1 d . . . . .
020 O 0.8009(10) -0.3987(6) 0.3213(7) 0.073(4) Uani 1 1 d . . . . .
P1 P 1.0000 -0.5000 0.5000 0.0111(5) Uani 1 2 d S . P . .
Mo1 Mo 1.21764(8) -0.50866(7) 0.21517(6) 0.02253(17) Uani 1 1 d . . . . .
Mo2 Mo 1.33050(8) -0.45547(7) 0.41464(8) 0.0314(2) Uani 1 1 d . . . . .
Mo3 Mo 1.07327(8) -0.24460(6) 0.33950(7) 0.02455(17) Uani 1 1 d . . . . .
Mo4 Mo 0.74251(8) -0.29391(7) 0.42318(7) 0.02804(19) Uani 1 1 d . . . . .
Mo5 Mo 0.89208(9) -0.56051(7) 0.30318(6) 0.02470(17) Uani 1 1 d . . . . .
Mo6 Mo 1.15553(7) -0.76709(6) 0.37601(6) 0.01962(16) Uani 1 1 d . . . . .
Ag1 Ag 0.5000 0.0000 0.5000 0.0600(5) Uani 1 2 d S . P . .
Ag2 Ag 0.81191(8) -0.03837(6) 0.20567(6) 0.03290(18) Uani 1 1 d . . . . .
Ag3 Ag 0.50835(8) 0.01051(6) 0.19944(7) 0.03325(18) Uani 1 1 d . . . . .
Ag4 Ag 1.0000 -0.5000 0.0000 0.0361(3) Uani 1 2 d S . P . .
Ag5 Ag 0.28739(9) -0.01921(6) 0.05367(7) 0.03552(19) Uani 1 1 d . . . . .
Ag6 Ag 0.61960(7) 0.49323(5) 0.14296(6) 0.02670(16) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
C1 N2 1.296(12) . ?
C1 N1 1.328(13) . ?
C1 H1 0.9300 . ?
C2 N3 1.312(13) . ?
C2 N1 1.340(13) . ?
C2 H2 0.9300 . ?
C3 N6 1.315(10) . ?
C3 N7 1.353(11) . ?
C3 H3 0.9300 . ?
C4 N5 1.321(11) . ?
C4 N7 1.339(11) . ?
C4 H4 0.9300 . ?
C5 N8 1.314(11) . ?
C5 N13 1.341(11) 1_545 ?
C5 H5 0.9300 . ?
C6 N9 1.317(11) . ?
C6 N13 1.338(11) 1_545 ?
C6 H6 0.9300 . ?
C7 N10 1.312(11) . ?
C7 N12 1.335(11) . ?
C7 H7 0.9300 . ?
C8 N11 1.319(12) . ?
C8 N12 1.322(12) . ?
C8 H8 0.9300 . ?
N2 N3 1.357(11) . ?
N2 Ag2 2.173(7) . ?
N3 Ag1 2.141(8) . ?
N5 N6 1.382(10) . ?
N5 Ag5 2.112(7) 2_655 ?
N6 Ag2 2.145(7) . ?
N7 Ag4 2.106(7) . ?
N8 N9 1.385(10) . ?
N8 Ag3 2.109(7) . ?
N9 Ag5 2.114(7) . ?
N10 N11 1.385(11) . ?
N10 Ag3 2.104(7) . ?
N11 Ag5 2.623(8) 2_655 ?
N12 Ag6 2.131(7) . ?
N13 C6 1.338(11) 1_565 ?
N13 C5 1.341(11) 1_565 ?
N13 Ag6 2.119(7) . ?
O21 Mo5 1.879(8) 2_746 ?
O21 Mo2 1.882(8) . ?
O22 Mo2 1.884(8) . ?
O22 Mo4 1.895(7) 2_746 ?
01 Mo2 1.649(6) . ?
02 Mo3 1.863(7) . ?
02 Mo2 1.947(8) . ?
03 Mo5 1.841(7) . ?
03 Mo6 1.960(6) . ?
04 Mo1 1.878(7) . ?
04 Mo6 1.904(7) . ?
05 Mo4 1.678(6) . ?
06 Mo3 1.874(7) . ?
06 Mo1 1.918(7) . ?
07 Mo1 1.903(6) . ?
07 Mo5 1.905(7) . ?
08 Mo6 1.831(7) . ?
08 Mo4 1.962(7) 2_746 ?
09 Mo3 1.660(6) . ?
010 Mo4 1.865(7) . ?
010 Mo3 1.918(6) . ?
011 Mo6 1.898(7) . ?
011 Mo3 1.929(7) 2_746 ?
012 Mo5 1.660(6) . ?
013 Mo1 1.643(7) . ?
014 Mo1 1.884(7) . ?
014 Mo2 1.894(8) . ?
015 Mo6 1.658(7) . ?
016 P1 1.520(10) . ?
016 017 1.684(14) 2_746 ?
016 018 1.775(15) . ?
016 Mo6 2.440(11) 2_746 ?
016 Mo4 2.500(10) . ?
016 Mo3 2.505(10) . ?
017 P1 1.505(11) . ?
017 016 1.684(14) 2_746 ?
017 018 1.728(14) . ?
017 019 1.798(15) . ?
017 Mo1 2.471(10) . ?
017 Mo5 2.482(10) . ?
017 Mo6 2.489(11) . ?
018 P1 1.553(11) . ?
018 Mo1 2.417(11) . ?
018 Mo3 2.444(10) . ?
018 Mo2 2.510(11) . ?
019 P1 1.596(10) . ?
019 Mo5 2.396(10) . ?
019 Mo4 2.422(11) . ?
019 Mo2 2.439(10) 2_746 ?
020 Mo4 1.824(7) . ?
020 Mo5 1.952(7) . ?
P1 017 1.505(11) 2_746 ?
P1 016 1.520(10) 2_746 ?
P1 018 1.553(11) 2_746 ?
P1 019 1.596(10) 2_746 ?
Mo2 019 2.439(10) 2_746 ?
Mo3 011 1.929(7) 2_746 ?
Mo4 O22 1.895(7) 2_746 ?
Mo4 08 1.962(7) 2_746 ?
Mo5 O21 1.879(8) 2_746 ?
Mo6 016 2.440(11) 2_746 ?
Ag1 N3 2.141(8) 2_656 ?
Ag2 Ag3 3.2604(11) . ?
Ag3 Ag5 3.1890(12) 2_655 ?
Ag4 N7 2.106(7) 2_745 ?
Ag5 N5 2.112(7) 2_655 ?
Ag5 N11 2.623(8) 2_655 ?
Ag5 Ag3 3.1890(12) 2_655 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
N2 C1 N1 111.4(9) . . ?
N2 C1 H1 124.3 . . ?
N1 C1 H1 124.3 . . ?
N3 C2 N1 108.6(9) . . ?
N3 C2 H2 125.7 . . ?
N1 C2 H2 125.7 . . ?
N6 C3 N7 111.3(7) . . ?
N6 C3 H3 124.4 . . ?
N7 C3 H3 124.4 . . ?
N5 C4 N7 112.5(8) . . ?
N5 C4 H4 123.7 . . ?
N7 C4 H4 123.7 . . ?
N8 C5 N13 112.9(8) . 1_545 ?
N8 C5 H5 123.6 . . ?
N13 C5 H5 123.6 1_545 . ?
N9 C6 N13 113.6(8) . 1_545 ?
N9 C6 H6 123.2 . . ?
N13 C6 H6 123.2 1_545 . ?
N10 C7 N12 112.4(8) . . ?
N10 C7 H7 123.8 . . ?
N12 C7 H7 123.8 . . ?
N11 C8 N12 113.8(8) . . ?
N11 C8 H8 123.1 . . ?
N12 C8 H8 123.1 . . ?
C1 N1 C2 105.7(8) . . ?
C1 N2 N3 105.9(7) . . ?
C1 N2 Ag2 126.1(6) . . ?
N3 N2 Ag2 128.0(6) . . ?
C2 N3 N2 108.4(8) . . ?
C2 N3 Ag1 123.6(7) . . ?
N2 N3 Ag1 127.7(6) . . ?
C4 N5 N6 105.4(7) . . ?
C4 N5 Ag5 130.6(7) . 2_655 ?
N6 N5 Ag5 123.6(5) . 2_655 ?
C3 N6 N5 107.0(7) . . ?
C3 N6 Ag2 123.9(6) . . ?
N5 N6 Ag2 128.0(5) . . ?
C4 N7 C3 103.8(7) . . ?
C4 N7 Ag4 130.3(6) . . ?
C3 N7 Ag4 125.9(6) . . ?
C5 N8 N9 106.1(7) . . ?
C5 N8 Ag3 129.1(6) . . ?
N9 N8 Ag3 120.7(5) . . ?
C6 N9 N8 104.9(7) . . ?
C6 N9 Ag5 128.4(6) . . ?
N8 N9 Ag5 126.5(5) . . ?
C7 N10 N11 106.4(7) . . ?
C7 N10 Ag3 140.2(7) . . ?
N11 N10 Ag3 112.7(5) . . ?
C8 N11 N10 104.3(7) . . ?
C8 N11 Ag5 133.1(7) . 2_655 ?
N10 N11 Ag5 107.0(5) . 2_655 ?
C8 N12 C7 103.1(7) . . ?
C8 N12 Ag6 125.8(6) . . ?
C7 N12 Ag6 128.9(6) . . ?
C6 N13 C5 102.5(7) 1_565 1_565 ?
C6 N13 Ag6 126.5(6) 1_565 . ?
C5 N13 Ag6 129.6(6) 1_565 . ?
Mo5 O21 Mo2 140.3(6) 2_746 . ?
Mo2 O22 Mo4 137.5(5) . 2_746 ?
Mo3 02 Mo2 137.8(5) . . ?
Mo5 03 Mo6 139.4(5) . . ?
Mo1 04 Mo6 141.1(5) . . ?
Mo3 06 Mo1 138.1(6) . . ?
Mo1 07 Mo5 136.3(4) . . ?
Mo6 08 Mo4 137.6(5) . 2_746 ?
Mo4 010 Mo3 142.6(5) . . ?
Mo6 011 Mo3 138.4(5) . 2_746 ?
Mo1 014 Mo2 141.0(5) . . ?
P1 016 017 55.7(5) . 2_746 ?
P1 016 018 55.6(5) . . ?
017 016 018 93.6(7) 2_746 . ?
P1 016 Mo6 127.3(6) . 2_746 ?
017 016 Mo6 71.6(5) 2_746 2_746 ?
018 016 Mo6 136.1(6) . 2_746 ?
P1 016 Mo4 121.6(5) . . ?
017 016 Mo4 131.5(6) 2_746 . ?
018 016 Mo4 125.9(6) . . ?
Mo6 016 Mo4 91.4(3) 2_746 . ?
P1 016 Mo3 122.7(6) . . ?
017 016 Mo3 133.1(6) 2_746 . ?
018 016 Mo3 67.2(5) . . ?
Mo6 016 Mo3 92.7(3) 2_746 . ?
Mo4 016 Mo3 91.4(3) . . ?
P1 017 016 56.6(5) . 2_746 ?
P1 017 018 56.9(5) . . ?
016 017 018 94.7(7) 2_746 . ?
P1 017 019 57.0(5) . . ?
016 017 019 92.5(7) 2_746 . ?
018 017 019 91.5(7) . . ?
P1 017 Mo1 124.6(6) . . ?
016 017 Mo1 133.6(7) 2_746 . ?
018 017 Mo1 67.6(5) . . ?
019 017 Mo1 128.7(6) . . ?
P1 017 Mo5 122.8(6) . . ?
016 017 Mo5 129.4(6) 2_746 . ?
018 017 Mo5 129.1(7) . . ?
019 017 Mo5 65.9(5) . . ?
Mo1 017 Mo5 91.1(3) . . ?
P1 017 Mo6 125.0(6) . . ?
016 017 Mo6 68.4(5) 2_746 . ?
018 017 Mo6 132.6(7) . . ?
019 017 Mo6 131.4(6) . . ?
Mo1 017 Mo6 91.9(4) . . ?
Mo5 017 Mo6 91.7(3) . . ?
P1 018 017 54.3(5) . . ?
P1 018 016 53.9(5) . . ?
017 018 016 91.7(7) . . ?
P1 018 Mo1 125.3(6) . . ?
017 018 Mo1 71.0(5) . . ?
016 018 Mo1 135.5(7) . . ?
P1 018 Mo3 124.7(6) . . ?
017 018 Mo3 136.3(7) . . ?
016 018 Mo3 70.8(5) . . ?
Mo1 018 Mo3 93.6(4) . . ?
P1 018 Mo2 120.1(6) . . ?
017 018 Mo2 128.5(7) . . ?
016 018 Mo2 128.1(6) . . ?
Mo1 018 Mo2 92.5(4) . . ?
Mo3 018 Mo2 91.7(4) . . ?
P1 019 017 52.2(5) . . ?
P1 019 Mo5 123.1(6) . . ?
017 019 Mo5 70.9(5) . . ?
P1 019 Mo4 122.3(6) . . ?
017 019 Mo4 132.2(6) . . ?
Mo5 019 Mo4 94.7(4) . . ?
P1 019 Mo2 122.0(6) . 2_746 ?
017 019 Mo2 132.3(7) . 2_746 ?
Mo5 019 Mo2 94.0(4) . 2_746 ?
Mo4 019 Mo2 92.8(4) . 2_746 ?
Mo4 020 Mo5 139.6(6) . . ?
017 P1 017 180.0 . 2_746 ?
017 P1 016 67.7(5) . 2_746 ?
017 P1 016 112.3(5) 2_746 2_746 ?
017 P1 016 112.3(5) . . ?
017 P1 016 67.7(5) 2_746 . ?
016 P1 016 180.0 2_746 . ?
017 P1 018 111.2(5) . 2_746 ?
017 P1 018 68.8(5) 2_746 2_746 ?
016 P1 018 70.6(5) 2_746 2_746 ?
016 P1 018 109.5(5) . 2_746 ?
017 P1 018 68.8(5) . . ?
017 P1 018 111.2(5) 2_746 . ?
016 P1 018 109.4(5) 2_746 . ?
016 P1 018 70.6(5) . . ?
018 P1 018 180.0 2_746 . ?
017 P1 019 109.2(5) . 2_746 ?
017 P1 019 70.8(5) 2_746 2_746 ?
016 P1 019 72.3(5) 2_746 2_746 ?
016 P1 019 107.7(5) . 2_746 ?
018 P1 019 106.7(6) 2_746 2_746 ?
018 P1 019 73.3(6) . 2_746 ?
017 P1 019 70.8(5) . . ?
017 P1 019 109.2(5) 2_746 . ?
016 P1 019 107.7(5) 2_746 . ?
016 P1 019 72.3(5) . . ?
018 P1 019 73.3(6) 2_746 . ?
018 P1 019 106.7(6) . . ?
019 P1 019 180.0 2_746 . ?
013 Mo1 04 102.1(4) . . ?
013 Mo1 014 101.8(4) . . ?
04 Mo1 014 89.0(3) . . ?
013 Mo1 07 101.4(4) . . ?
04 Mo1 07 87.9(3) . . ?
014 Mo1 07 156.7(4) . . ?
013 Mo1 06 100.7(4) . . ?
04 Mo1 06 157.2(4) . . ?
014 Mo1 06 86.6(3) . . ?
07 Mo1 06 87.4(3) . . ?
013 Mo1 018 158.5(4) . . ?
04 Mo1 018 94.2(4) . . ?
014 Mo1 018 64.2(4) . . ?
07 Mo1 018 93.0(4) . . ?
06 Mo1 018 63.8(4) . . ?
013 Mo1 017 160.2(4) . . ?
04 Mo1 017 63.7(4) . . ?
014 Mo1 017 92.1(4) . . ?
07 Mo1 017 65.9(3) . . ?
06 Mo1 017 94.2(4) . . ?
018 Mo1 017 41.4(3) . . ?
01 Mo2 O21 102.0(4) . . ?
01 Mo2 O22 102.1(4) . . ?
O21 Mo2 O22 89.6(3) . . ?
01 Mo2 014 102.7(4) . . ?
O21 Mo2 014 155.1(5) . . ?
O22 Mo2 014 88.3(4) . . ?
01 Mo2 02 101.2(4) . . ?
O21 Mo2 02 85.5(4) . . ?
O22 Mo2 02 156.6(5) . . ?
014 Mo2 02 86.6(3) . . ?
01 Mo2 019 157.7(3) . 2_746 ?
O21 Mo2 019 62.1(4) . 2_746 ?
O22 Mo2 019 64.2(4) . 2_746 ?
014 Mo2 019 94.8(4) . 2_746 ?
02 Mo2 019 93.5(4) . 2_746 ?
01 Mo2 018 157.7(3) . . ?
O21 Mo2 018 93.4(5) . . ?
O22 Mo2 018 93.9(4) . . ?
014 Mo2 018 62.0(4) . . ?
02 Mo2 018 63.7(4) . . ?
019 Mo2 018 44.6(3) 2_746 . ?
09 Mo3 02 103.0(4) . . ?
09 Mo3 06 102.2(4) . . ?
02 Mo3 06 90.2(3) . . ?
09 Mo3 010 101.6(4) . . ?
02 Mo3 010 155.2(4) . . ?
06 Mo3 010 87.9(3) . . ?
09 Mo3 011 101.1(4) . 2_746 ?
02 Mo3 011 86.6(4) . 2_746 ?
06 Mo3 011 156.6(4) . 2_746 ?
010 Mo3 011 85.5(3) . 2_746 ?
09 Mo3 018 161.0(4) . . ?
02 Mo3 018 66.1(4) . . ?
06 Mo3 018 63.7(4) . . ?
010 Mo3 018 91.1(4) . . ?
011 Mo3 018 94.0(4) 2_746 . ?
09 Mo3 016 156.9(4) . . ?
02 Mo3 016 92.9(4) . . ?
06 Mo3 016 94.2(4) . . ?
010 Mo3 016 62.6(3) . . ?
011 Mo3 016 62.9(4) 2_746 . ?
018 Mo3 016 42.0(3) . . ?
05 Mo4 020 103.0(4) . . ?
05 Mo4 010 100.4(4) . . ?
020 Mo4 010 90.9(4) . . ?
05 Mo4 O22 103.1(4) . 2_746 ?
020 Mo4 O22 89.5(3) . 2_746 ?
010 Mo4 O22 155.7(5) . 2_746 ?
05 Mo4 08 99.5(4) . 2_746 ?
020 Mo4 08 157.4(5) . 2_746 ?
010 Mo4 08 85.9(3) . 2_746 ?
O22 Mo4 08 84.4(4) 2_746 2_746 ?
05 Mo4 019 160.1(3) . . ?
020 Mo4 019 63.1(4) . . ?
010 Mo4 019 94.2(4) . . ?
O22 Mo4 019 64.5(4) 2_746 . ?
08 Mo4 019 94.8(4) 2_746 . ?
05 Mo4 016 156.1(3) . . ?
020 Mo4 016 95.0(5) . . ?
010 Mo4 016 63.2(3) . . ?
O22 Mo4 016 92.5(4) 2_746 . ?
08 Mo4 016 63.6(4) 2_746 . ?
019 Mo4 016 43.8(3) . . ?
012 Mo5 03 101.6(4) . . ?
012 Mo5 O21 101.8(5) . 2_746 ?
03 Mo5 O21 90.0(4) . 2_746 ?
012 Mo5 07 100.7(4) . . ?
03 Mo5 07 89.6(3) . . ?
O21 Mo5 07 157.2(4) 2_746 . ?
012 Mo5 020 101.2(4) . . ?
03 Mo5 020 157.2(4) . . ?
O21 Mo5 020 85.8(3) 2_746 . ?
07 Mo5 020 85.7(3) . . ?
012 Mo5 019 157.0(4) . . ?
03 Mo5 019 95.9(4) . . ?
O21 Mo5 019 63.1(4) 2_746 . ?
07 Mo5 019 94.2(4) . . ?
020 Mo5 019 62.3(4) . . ?
012 Mo5 017 159.8(4) . . ?
03 Mo5 017 65.0(4) . . ?
O21 Mo5 017 93.6(5) 2_746 . ?
07 Mo5 017 65.7(3) . . ?
020 Mo5 017 92.9(4) . . ?
019 Mo5 017 43.2(3) . . ?
015 Mo6 08 103.0(4) . . ?
015 Mo6 011 102.9(4) . . ?
08 Mo6 011 91.2(3) . . ?
015 Mo6 04 101.4(4) . . ?
08 Mo6 04 89.9(3) . . ?
011 Mo6 04 154.8(4) . . ?
015 Mo6 03 100.6(4) . . ?
08 Mo6 03 156.3(4) . . ?
011 Mo6 03 84.7(3) . . ?
04 Mo6 03 84.3(3) . . ?
015 Mo6 016 162.5(4) . 2_746 ?
08 Mo6 016 66.5(4) . 2_746 ?
011 Mo6 016 64.7(4) . 2_746 ?
04 Mo6 016 92.9(4) . 2_746 ?
03 Mo6 016 90.8(4) . 2_746 ?
015 Mo6 017 157.5(4) . . ?
08 Mo6 017 93.5(4) . . ?
011 Mo6 017 91.8(4) . . ?
04 Mo6 017 63.0(4) . . ?
03 Mo6 017 63.5(3) . . ?
016 Mo6 017 39.9(3) 2_746 . ?
N3 Ag1 N3 180.0 2_656 . ?
N6 Ag2 N2 168.3(3) . . ?
N6 Ag2 Ag3 83.0(2) . . ?
N2 Ag2 Ag3 105.14(19) . . ?
N10 Ag3 N8 160.5(3) . . ?
N10 Ag3 Ag5 74.1(2) . 2_655 ?
N8 Ag3 Ag5 88.1(2) . 2_655 ?
N10 Ag3 Ag2 61.6(2) . . ?
N8 Ag3 Ag2 106.3(2) . . ?
Ag5 Ag3 Ag2 73.86(3) 2_655 . ?
N7 Ag4 N7 180.0 . 2_745 ?
N5 Ag5 N9 166.4(3) 2_655 . ?
N5 Ag5 N11 98.0(3) 2_655 2_655 ?
N9 Ag5 N11 92.3(3) . 2_655 ?
N5 Ag5 Ag3 84.7(2) 2_655 2_655 ?
N9 Ag5 Ag3 92.9(2) . 2_655 ?
N11 Ag5 Ag3 59.63(18) 2_655 2_655 ?
N13 Ag6 N12 168.2(3) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
N2 C1 N1 C2 -0.6(14) . . . . ?
N3 C2 N1 C1 0.7(14) . . . . ?
N1 C1 N2 N3 0.2(13) . . . . ?
N1 C1 N2 Ag2 -179.1(7) . . . . ?
N1 C2 N3 N2 -0.5(14) . . . . ?
N1 C2 N3 Ag1 173.5(8) . . . . ?
C1 N2 N3 C2 0.2(12) . . . . ?
Ag2 N2 N3 C2 179.5(8) . . . . ?
C1 N2 N3 Ag1 -173.6(8) . . . . ?
Ag2 N2 N3 Ag1 5.7(13) . . . . ?
N7 C4 N5 N6 1.9(12) . . . . ?
N7 C4 N5 Ag5 -171.3(7) . . . 2_655 ?
N7 C3 N6 N5 0.1(11) . . . . ?
N7 C3 N6 Ag2 169.0(6) . . . . ?
C4 N5 N6 C3 -1.2(11) . . . . ?
Ag5 N5 N6 C3 172.7(6) 2_655 . . . ?
C4 N5 N6 Ag2 -169.5(7) . . . . ?
Ag5 N5 N6 Ag2 4.4(11) 2_655 . . . ?
N5 C4 N7 C3 -1.8(12) . . . . ?
N5 C4 N7 Ag4 -180.0(7) . . . . ?
N6 C3 N7 C4 1.0(11) . . . . ?
N6 C3 N7 Ag4 179.3(6) . . . . ?
N13 C5 N8 N9 -1.0(10) 1_545 . . . ?
N13 C5 N8 Ag3 -157.8(6) 1_545 . . . ?
N13 C6 N9 N8 -0.7(12) 1_545 . . . ?
N13 C6 N9 Ag5 -175.7(7) 1_545 . . . ?
C5 N8 N9 C6 1.0(10) . . . . ?
Ag3 N8 N9 C6 160.1(7) . . . . ?
C5 N8 N9 Ag5 176.1(6) . . . . ?
Ag3 N8 N9 Ag5 -24.8(10) . . . . ?
N12 C7 N10 N11 0.2(11) . . . . ?
N12 C7 N10 Ag3 -168.3(7) . . . . ?
N12 C8 N11 N10 0.4(12) . . . . ?
N12 C8 N11 Ag5 131.2(8) . . . 2_655 ?
C7 N10 N11 C8 -0.4(11) . . . . ?
Ag3 N10 N11 C8 171.7(7) . . . . ?
C7 N10 N11 Ag5 -145.0(6) . . . 2_655 ?
Ag3 N10 N11 Ag5 27.0(6) . . . 2_655 ?
N11 C8 N12 C7 -0.3(12) . . . . ?
N11 C8 N12 Ag6 -164.5(7) . . . . ?
N10 C7 N12 C8 0.1(11) . . . . ?
N10 C7 N12 Ag6 163.5(6) . . . . ?
016 017 018 P1 -44.6(5) 2_746 . . . ?
019 017 018 P1 48.1(5) . . . . ?
Mo1 017 018 P1 179.8(5) . . . . ?
Mo5 017 018 P1 107.7(8) . . . . ?
Mo6 017 018 P1 -109.4(8) . . . . ?
P1 017 018 016 -41.6(5) . . . . ?
016 017 018 016 -86.2(7) 2_746 . . . ?
019 017 018 016 6.4(7) . . . . ?
Mo1 017 018 016 138.2(6) . . . . ?
Mo5 017 018 016 66.1(9) . . . . ?
Mo6 017 018 016 -151.0(8) . . . . ?
P1 017 018 Mo1 -179.8(5) . . . . ?
016 017 018 Mo1 135.6(6) 2_746 . . . ?
019 017 018 Mo1 -131.7(6) . . . . ?
Mo5 017 018 Mo1 -72.1(7) . . . . ?
Mo6 017 018 Mo1 70.8(7) . . . . ?
P1 017 018 Mo3 -105.2(9) . . . . ?
016 017 018 Mo3 -149.8(9) 2_746 . . . ?
019 017 018 Mo3 -57.1(10) . . . . ?
Mo1 017 018 Mo3 74.6(8) . . . . ?
Mo5 017 018 Mo3 2.5(14) . . . . ?
Mo6 017 018 Mo3 145.4(7) . . . . ?
P1 017 018 Mo2 102.5(8) . . . . ?
016 017 018 Mo2 58.0(9) 2_746 . . . ?
019 017 018 Mo2 150.6(7) . . . . ?
Mo1 017 018 Mo2 -77.7(7) . . . . ?
Mo5 017 018 Mo2 -149.7(6) . . . . ?
Mo6 017 018 Mo2 -6.8(13) . . . . ?
017 016 018 P1 43.3(5) 2_746 . . . ?
Mo6 016 018 P1 110.4(9) 2_746 . . . ?
Mo4 016 018 P1 -106.7(7) . . . . ?
Mo3 016 018 P1 179.1(5) . . . . ?
P1 016 018 017 41.9(5) . . . . ?
017 016 018 017 85.2(7) 2_746 . . . ?
Mo6 016 018 017 152.3(8) 2_746 . . . ?
Mo4 016 018 017 -64.8(8) . . . . ?
Mo3 016 018 017 -139.1(6) . . . . ?
P1 016 018 Mo1 106.1(9) . . . . ?
017 016 018 Mo1 149.4(8) 2_746 . . . ?
Mo6 016 018 Mo1 -143.5(7) 2_746 . . . ?
Mo4 016 018 Mo1 -0.7(13) . . . . ?
Mo3 016 018 Mo1 -74.9(8) . . . . ?
P1 016 018 Mo3 -179.1(5) . . . . ?
017 016 018 Mo3 -135.7(6) 2_746 . . . ?
Mo6 016 018 Mo3 -68.6(8) 2_746 . . . ?
Mo4 016 018 Mo3 74.2(6) . . . . ?
P1 016 018 Mo2 -102.5(7) . . . . ?
017 016 018 Mo2 -59.2(9) 2_746 . . . ?
Mo6 016 018 Mo2 7.9(13) 2_746 . . . ?
Mo4 016 018 Mo2 150.8(5) . . . . ?
Mo3 016 018 Mo2 76.5(6) . . . . ?
016 017 019 P1 46.7(5) 2_746 . . . ?
018 017 019 P1 -48.0(5) . . . . ?
Mo1 017 019 P1 -110.2(8) . . . . ?
Mo5 017 019 P1 179.2(5) . . . . ?
Mo6 017 019 P1 109.9(8) . . . . ?
P1 017 019 Mo5 -179.2(5) . . . . ?
016 017 019 Mo5 -132.5(6) 2_746 . . . ?
018 017 019 Mo5 132.7(6) . . . . ?
Mo1 017 019 Mo5 70.5(6) . . . . ?
Mo6 017 019 Mo5 -69.4(7) . . . . ?
P1 017 019 Mo4 102.1(8) . . . . ?
016 017 019 Mo4 148.8(7) 2_746 . . . ?
018 017 019 Mo4 54.1(9) . . . . ?
Mo1 017 019 Mo4 -8.2(12) . . . . ?
Mo5 017 019 Mo4 -78.7(7) . . . . ?
Mo6 017 019 Mo4 -148.0(6) . . . . ?
P1 017 019 Mo2 -101.6(8) . . . 2_746 ?
016 017 019 Mo2 -54.9(9) 2_746 . . 2_746 ?
018 017 019 Mo2 -149.6(8) . . . 2_746 ?
Mo1 017 019 Mo2 148.2(6) . . . 2_746 ?
Mo5 017 019 Mo2 77.6(7) . . . 2_746 ?
Mo6 017 019 Mo2 8.3(13) . . . 2_746 ?
018 017 P1 016 -123.1(7) . . . 2_746 ?
019 017 P1 016 119.4(6) . . . 2_746 ?
Mo1 017 P1 016 -123.3(8) . . . 2_746 ?
Mo5 017 P1 016 118.6(8) . . . 2_746 ?
Mo6 017 P1 016 -1.1(6) . . . 2_746 ?
016 017 P1 016 179.999(1) 2_746 . . . ?
018 017 P1 016 56.9(7) . . . . ?
019 017 P1 016 -60.6(6) . . . . ?
Mo1 017 P1 016 56.7(8) . . . . ?
Mo5 017 P1 016 -61.4(8) . . . . ?
Mo6 017 P1 016 178.9(6) . . . . ?
016 017 P1 018 -56.9(7) 2_746 . . 2_746 ?
018 017 P1 018 180.001(1) . . . 2_746 ?
019 017 P1 018 62.5(7) . . . 2_746 ?
Mo1 017 P1 018 179.8(6) . . . 2_746 ?
Mo5 017 P1 018 61.7(8) . . . 2_746 ?
Mo6 017 P1 018 -58.0(8) . . . 2_746 ?
016 017 P1 018 123.1(7) 2_746 . . . ?
019 017 P1 018 -117.5(7) . . . . ?
Mo1 017 P1 018 -0.2(6) . . . . ?
Mo5 017 P1 018 -118.3(8) . . . . ?
Mo6 017 P1 018 122.0(8) . . . . ?
016 017 P1 019 60.6(6) 2_746 . . 2_746 ?
018 017 P1 019 -62.5(7) . . . 2_746 ?
019 017 P1 019 180.002(2) . . . 2_746 ?
Mo1 017 P1 019 -62.7(8) . . . 2_746 ?
Mo5 017 P1 019 179.2(6) . . . 2_746 ?
Mo6 017 P1 019 59.5(8) . . . 2_746 ?
016 017 P1 019 -119.4(6) 2_746 . . . ?
018 017 P1 019 117.5(7) . . . . ?
Mo1 017 P1 019 117.3(8) . . . . ?
Mo5 017 P1 019 -0.8(6) . . . . ?
Mo6 017 P1 019 -120.5(8) . . . . ?
017 016 P1 017 180.001(1) 2_746 . . . ?
018 016 P1 017 -56.0(7) . . . . ?
Mo6 016 P1 017 178.9(6) 2_746 . . . ?
Mo4 016 P1 017 58.5(8) . . . . ?
Mo3 016 P1 017 -57.0(8) . . . . ?
018 016 P1 017 124.0(7) . . . 2_746 ?
Mo6 016 P1 017 -1.1(6) 2_746 . . 2_746 ?
Mo4 016 P1 017 -121.5(8) . . . 2_746 ?
Mo3 016 P1 017 123.0(8) . . . 2_746 ?
017 016 P1 018 56.0(7) 2_746 . . 2_746 ?
018 016 P1 018 179.999(1) . . . 2_746 ?
Mo6 016 P1 018 54.8(8) 2_746 . . 2_746 ?
Mo4 016 P1 018 -65.5(7) . . . 2_746 ?
Mo3 016 P1 018 179.0(6) . . . 2_746 ?
017 016 P1 018 -124.0(7) 2_746 . . . ?
Mo6 016 P1 018 -125.2(8) 2_746 . . . ?
Mo4 016 P1 018 114.5(7) . . . . ?
Mo3 016 P1 018 -1.0(6) . . . . ?
017 016 P1 019 -59.7(6) 2_746 . . 2_746 ?
018 016 P1 019 64.3(6) . . . 2_746 ?
Mo6 016 P1 019 -60.8(8) 2_746 . . 2_746 ?
Mo4 016 P1 019 178.8(6) . . . 2_746 ?
Mo3 016 P1 019 63.3(7) . . . 2_746 ?
017 016 P1 019 120.3(6) 2_746 . . . ?
018 016 P1 019 -115.7(6) . . . . ?
Mo6 016 P1 019 119.2(8) 2_746 . . . ?
Mo4 016 P1 019 -1.2(6) . . . . ?
Mo3 016 P1 019 -116.7(7) . . . . ?
016 018 P1 017 124.7(7) . . . . ?
Mo1 018 P1 017 0.2(6) . . . . ?
Mo3 018 P1 017 125.8(8) . . . . ?
Mo2 018 P1 017 -118.0(7) . . . . ?
017 018 P1 017 179.998(1) . . . 2_746 ?
016 018 P1 017 -55.3(7) . . . 2_746 ?
Mo1 018 P1 017 -179.8(6) . . . 2_746 ?
Mo3 018 P1 017 -54.2(8) . . . 2_746 ?
Mo2 018 P1 017 62.0(7) . . . 2_746 ?
017 018 P1 016 55.3(7) . . . 2_746 ?
016 018 P1 016 180.000(1) . . . 2_746 ?
Mo1 018 P1 016 55.5(8) . . . 2_746 ?
Mo3 018 P1 016 -178.9(6) . . . 2_746 ?
Mo2 018 P1 016 -62.7(7) . . . 2_746 ?
017 018 P1 016 -124.7(7) . . . . ?
Mo1 018 P1 016 -124.5(8) . . . . ?
Mo3 018 P1 016 1.1(6) . . . . ?
Mo2 018 P1 016 117.3(7) . . . . ?
017 018 P1 019 119.0(6) . . . 2_746 ?
016 018 P1 019 -116.3(6) . . . 2_746 ?
Mo1 018 P1 019 119.2(8) . . . 2_746 ?
Mo3 018 P1 019 -115.2(8) . . . 2_746 ?
Mo2 018 P1 019 1.0(6) . . . 2_746 ?
017 018 P1 019 -61.0(6) . . . . ?
016 018 P1 019 63.7(6) . . . . ?
Mo1 018 P1 019 -60.8(8) . . . . ?
Mo3 018 P1 019 64.8(8) . . . . ?
Mo2 018 P1 019 -179.0(6) . . . . ?
Mo5 019 P1 017 0.9(6) . . . . ?
Mo4 019 P1 017 -121.0(8) . . . . ?
Mo2 019 P1 017 121.4(8) 2_746 . . . ?
017 019 P1 017 180.000(2) . . . 2_746 ?
Mo5 019 P1 017 -179.1(6) . . . 2_746 ?
Mo4 019 P1 017 59.0(8) . . . 2_746 ?
Mo2 019 P1 017 -58.6(8) 2_746 . . 2_746 ?
017 019 P1 016 -57.7(6) . . . 2_746 ?
Mo5 019 P1 016 -56.9(8) . . . 2_746 ?
Mo4 019 P1 016 -178.7(6) . . . 2_746 ?
Mo2 019 P1 016 63.6(7) 2_746 . . 2_746 ?
017 019 P1 016 122.3(6) . . . . ?
Mo5 019 P1 016 123.1(8) . . . . ?
Mo4 019 P1 016 1.2(6) . . . . ?
Mo2 019 P1 016 -116.4(7) 2_746 . . . ?
017 019 P1 018 -120.3(6) . . . 2_746 ?
Mo5 019 P1 018 -119.4(8) . . . 2_746 ?
Mo4 019 P1 018 118.7(7) . . . 2_746 ?
Mo2 019 P1 018 1.1(6) 2_746 . . 2_746 ?
017 019 P1 018 59.7(6) . . . . ?
Mo5 019 P1 018 60.6(8) . . . . ?
Mo4 019 P1 018 -61.3(7) . . . . ?
Mo2 019 P1 018 -178.9(6) 2_746 . . . ?
Mo6 04 Mo1 013 -159.9(7) . . . . ?
Mo6 04 Mo1 014 98.3(7) . . . . ?
Mo6 04 Mo1 07 -58.6(7) . . . . ?
Mo6 04 Mo1 06 19.6(13) . . . . ?
Mo6 04 Mo1 018 34.3(7) . . . . ?
Mo6 04 Mo1 017 5.4(6) . . . . ?
Mo2 014 Mo1 013 157.6(8) . . . . ?
Mo2 014 Mo1 04 -100.3(8) . . . . ?
Mo2 014 Mo1 07 -18.0(14) . . . . ?
Mo2 014 Mo1 06 57.4(8) . . . . ?
Mo2 014 Mo1 018 -5.1(7) . . . . ?
Mo2 014 Mo1 017 -36.7(8) . . . . ?
Mo5 O21 Mo2 01 -155.9(9) 2_746 . . . ?
Mo5 O21 Mo2 O22 -53.5(10) 2_746 . . . ?
Mo5 O21 Mo2 014 31.5(15) 2_746 . . . ?
Mo5 O21 Mo2 02 103.6(10) 2_746 . . . ?
Mo5 O21 Mo2 019 7.3(8) 2_746 . . 2_746 ?
Mo5 O21 Mo2 018 40.4(10) 2_746 . . . ?
Mo4 O22 Mo2 01 150.5(8) 2_746 . . . ?
Mo4 O22 Mo2 O21 48.2(9) 2_746 . . . ?
Mo4 O22 Mo2 014 -106.9(9) 2_746 . . . ?
Mo4 O22 Mo2 02 -29.5(15) 2_746 . . . ?
Mo4 O22 Mo2 019 -10.7(8) 2_746 . . 2_746 ?
Mo4 O22 Mo2 018 -45.1(9) 2_746 . . . ?
Mo1 014 Mo2 01 -157.6(8) . . . . ?
Mo1 014 Mo2 O21 15.0(14) . . . . ?
Mo1 014 Mo2 O22 100.3(8) . . . . ?
Mo1 014 Mo2 02 -56.8(8) . . . . ?
Mo1 014 Mo2 019 36.4(8) . . . 2_746 ?
Mo1 014 Mo2 018 5.0(7) . . . . ?
Mo2 02 Mo3 09 -154.0(8) . . . . ?
Mo2 02 Mo3 06 -51.5(9) . . . . ?
Mo2 02 Mo3 010 33.9(14) . . . . ?
Mo2 02 Mo3 011 105.3(8) . . . 2_746 ?
Mo2 02 Mo3 018 9.5(7) . . . . ?
Mo2 02 Mo3 016 42.7(8) . . . . ?
Mo1 06 Mo3 09 156.3(7) . . . . ?
Mo1 06 Mo3 02 52.9(8) . . . . ?
Mo1 06 Mo3 010 -102.3(7) . . . . ?
Mo1 06 Mo3 011 -28.9(13) . . . 2_746 ?
Mo1 06 Mo3 018 -10.1(6) . . . . ?
Mo1 06 Mo3 016 -40.0(7) . . . . ?
Mo5 020 Mo4 05 -158.3(8) . . . . ?
Mo5 020 Mo4 010 100.8(8) . . . . ?
Mo5 020 Mo4 O22 -54.9(9) . . . 2_746 ?
Mo5 020 Mo4 08 19.2(14) . . . 2_746 ?
Mo5 020 Mo4 019 6.5(7) . . . . ?
Mo5 020 Mo4 016 37.6(8) . . . . ?
Mo3 010 Mo4 05 158.1(8) . . . . ?
Mo3 010 Mo4 020 -98.4(9) . . . . ?
Mo3 010 Mo4 O22 -7.6(15) . . . 2_746 ?
Mo3 010 Mo4 08 59.2(8) . . . 2_746 ?
Mo3 010 Mo4 019 -35.3(8) . . . . ?
Mo3 010 Mo4 016 -3.3(7) . . . . ?
Mo6 03 Mo5 012 156.3(7) . . . . ?
Mo6 03 Mo5 O21 -101.7(8) . . . 2_746 ?
Mo6 03 Mo5 07 55.5(7) . . . . ?
Mo6 03 Mo5 020 -22.5(13) . . . . ?
Mo6 03 Mo5 019 -38.7(7) . . . . ?
Mo6 03 Mo5 017 -7.6(6) . . . . ?
Mo4 08 Mo6 015 -155.2(7) 2_746 . . . ?
Mo4 08 Mo6 011 -51.7(7) 2_746 . . . ?
Mo4 08 Mo6 04 103.1(7) 2_746 . . . ?
Mo4 08 Mo6 03 27.7(12) 2_746 . . . ?
Mo4 08 Mo6 016 9.9(6) 2_746 . . 2_746 ?
Mo4 08 Mo6 017 40.2(7) 2_746 . . . ?
Mo3 011 Mo6 015 154.0(7) 2_746 . . . ?
Mo3 011 Mo6 08 50.3(7) 2_746 . . . ?
Mo3 011 Mo6 04 -41.9(11) 2_746 . . . ?
Mo3 011 Mo6 03 -106.3(7) 2_746 . . . ?
Mo3 011 Mo6 016 -12.9(6) 2_746 . . 2_746 ?
Mo3 011 Mo6 017 -43.2(7) 2_746 . . . ?

_refine_diff_density_max         1.440
_refine_diff_density_min         -1.294
_refine_diff_density_rms         0.222

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_shelx
_database_code_depnum_ccdc_archive 'CCDC 1494914'
_audit_update_record             
;
2016-07-20 deposited with the CCDC.
2016-10-28 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2014/7
_shelx_SHELXL_version_number     2014/7
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         'C12 H12 Ag5 Mo12 N18 O40 P'
_chemical_formula_sum            'C12 H12 Ag5 Mo12 N18 O40 P'
_chemical_formula_weight         2770.00

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ag Ag -0.8971 1.1015 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      trigonal
_space_group_IT_number           162
_space_group_name_H-M_alt        'P -3 1 m'
_space_group_name_Hall           '-P 3 2'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-y, -x, -z'
'x, x-y, -z'
'-x+y, y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'y, x, z'
'-x, -x+y, z'
'x-y, -y, z'

_cell_length_a                   12.1615(3)
_cell_length_b                   12.1615(3)
_cell_length_c                   10.4558(5)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_volume                     1339.25(11)
_cell_formula_units_Z            1
_cell_measurement_temperature    273(2)
_cell_measurement_reflns_used    10628
_cell_measurement_theta_min      3.350
_cell_measurement_theta_max      29.282

_exptl_crystal_description       block
_exptl_crystal_colour            yellow
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    3.435
_exptl_crystal_F_000             1284
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          ?
_exptl_crystal_size_mid          ?
_exptl_crystal_size_min          ?
_exptl_absorpt_coefficient_mu    4.630
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      273(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'multiwire proportional'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            10628
_diffrn_reflns_av_unetI/netI     0.0265
_diffrn_reflns_av_R_equivalents  0.0410
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_theta_min         3.350
_diffrn_reflns_theta_max         29.282
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.952
_diffrn_measured_fraction_theta_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.952
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.952
_diffrn_reflns_point_group_measured_fraction_full 0.997
_reflns_number_total             1262
_reflns_number_gt                1053
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker FRAMBO'
_computing_cell_refinement       'Bruker FRAMBO'
_computing_data_reduction        'Bruker SHELXTL'
_computing_structure_solution    'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0432P)²+24.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_extinction_coef       0.0014(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         1262
_refine_ls_number_parameters     109
_refine_ls_number_restraints     123
_refine_ls_R_factor_all          0.0670
_refine_ls_R_factor_gt           0.0534
_refine_ls_wR_factor_ref         0.1291
_refine_ls_wR_factor_gt          0.1224
_refine_ls_goodness_of_fit_ref   1.036
_refine_ls_restrained_S_all      1.055
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.83216(8) 0.83216(8) 0.27671(9) 0.0326(3) Uani 1 2 d S TU P . .
Mo2 Mo 0.66409(9) 0.83205(4) 0.0000 0.0312(3) Uani 1 2 d S TU P . .
P1 P 1.0000 1.0000 0.0000 0.0160(11) Uani 1 12 d S TU P . .
O4 O 0.5077(8) 0.7538(4) 0.0000 0.047(2) Uani 1 2 d S TU P . .
O2 O 0.7525(8) 0.7525(8) 0.4045(8) 0.053(2) Uani 1 2 d S TU P . .
O3 O 0.6976(8) 0.8213(8) 0.1755(6) 0.061(2) Uani 1 1 d . U . . .
O9 O 0.7004(10) 1.0000 0.0295(9) 0.058(3) Uani 1 2 d S TU P . .
O1 O 1.0000 0.8746(8) 0.3184(12) 0.059(3) Uani 1 2 d S TU P . .
O6 O 0.8816(11) 0.8816(11) 0.0483(13) 0.023(2) Uani 0.5 2 d S TU P . .
O5 O 1.0000 1.0000 -0.145(2) 0.021(4) Uani 0.5 6 d S TU P . .
Ag1 Ag 0.3333 0.6667 0.7815(3) 0.0529(7) Uani 0.5 3 d S TU P . .
Ag2 Ag 0.77660(12) 0.5532(2) 0.5000 0.0538(6) Uani 0.5 2 d S TU P . .
N1 N 0.4578(19) 0.586(2) 0.7242(19) 0.043(4) Uani 0.5 1 d . U P A -1
N2 N 0.578(2) 0.498(2) 0.729(2) 0.047(5) Uani 0.5 1 d . U P A -1
N3 N 0.6208(17) 0.5810(17) 0.6296(16) 0.048(4) Uani 0.5 1 d . U P A -1
C1 C 0.4835(16) 0.5050(18) 0.7828(17) 0.044(4) Uani 0.5 1 d . U P A -1
H1 H 0.4396 0.4579 0.8543 0.053 Uiso 0.5 1 calc R U P A -1
C2 C 0.5426(19) 0.640(2) 0.6300(19) 0.040(4) Uani 0.5 1 d . U P A -1
H2 H 0.5500 0.7034 0.5751 0.047 Uiso 0.5 1 calc R U P A -1


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O2 1.650(8) . ?
Mo1 O1 1.889(4) . ?
Mo1 O1 1.889(4) 3_675 ?
Mo1 O3 1.897(7) . ?
Mo1 O3 1.897(7) 10 ?
Mo1 O6 2.462(13) . ?
Mo1 O5 2.463(13) 7_775 ?
Mo2 O4 1.647(8) . ?
Mo2 O9 1.887(4) 9_655 ?
Mo2 O9 1.887(4) . ?
Mo2 O3 1.898(6) . ?
Mo2 O3 1.898(6) 5_565 ?
Mo2 O6 2.454(9) . ?
Mo2 O6 2.454(10) 8_565 ?
P1 O5 1.52(2) 7_775 ?
P1 O5 1.52(2) . ?
P1 O6 1.526(14) 9_655 ?
P1 O6 1.526(14) 7_775 ?
P1 O6 1.526(14) 2_765 ?
P1 O6 1.526(14) 8_565 ?
P1 O6 1.526(14) 3_675 ?
P1 O6 1.526(14) . ?
O9 Mo2 1.887(4) 8_565 ?
O1 Mo1 1.889(4) 2_765 ?
O6 O5 1.759(19) 7_775 ?
O6 O6 1.759(19) 9_655 ?
O6 O6 1.759(19) 8_565 ?
O6 Mo2 2.454(9) 9_655 ?
O5 O6 1.759(19) 7_775 ?
O5 O6 1.759(19) 9_655 ?
O5 O6 1.759(19) 8_565 ?
O5 Mo1 2.463(12) 8_565 ?
O5 Mo1 2.463(12) 9_655 ?
O5 Mo1 2.463(12) 7_775 ?
Ag1 N1 2.26(2) . ?
Ag1 N2 2.762(19) 11_665 ?
Ag2 N3 2.486(17) 6_656 ?
Ag2 N3 2.486(17) . ?
N1 C1 1.32(3) . ?
N1 C2 1.34(3) . ?
N2 C1 1.32(3) . ?
N2 N3 1.36(2) . ?
N2 Ag1 2.762(19) 12_665 ?
N3 C2 1.45(3) . ?
C1 H1 0.9300 . ?
C2 H2 0.9300 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Mo1 O1 102.2(4) . . ?
O2 Mo1 O1 102.2(4) . 3_675 ?
O1 Mo1 O1 88.7(6) . 3_675 ?
O2 Mo1 O3 100.3(4) . . ?
O1 Mo1 O3 157.5(5) . . ?
O1 Mo1 O3 87.9(4) 3_675 . ?
O2 Mo1 O3 100.3(4) . 10 ?
O1 Mo1 O3 87.9(4) . 10 ?
O1 Mo1 O3 157.5(5) 3_675 10 ?
O3 Mo1 O3 86.7(4) . 10 ?
O2 Mo1 O6 158.2(5) . . ?
O1 Mo1 O6 93.4(4) . . ?
O1 Mo1 O6 93.4(4) 3_675 . ?
O3 Mo1 O6 64.7(3) . . ?
O3 Mo1 O6 64.7(3) 10 . ?
O2 Mo1 O5 160.0(6) . 7_775 ?
O1 Mo1 O5 64.4(4) . 7_775 ?
O1 Mo1 O5 64.4(4) 3_675 7_775 ?
O3 Mo1 O5 94.2(4) . 7_775 ?
O3 Mo1 O5 94.2(4) 10 7_775 ?
O6 Mo1 O5 41.8(5) . 7_775 ?
O4 Mo2 O9 101.7(4) . 9_655 ?
O4 Mo2 O9 101.7(4) . . ?
O9 Mo2 O9 156.6(7) 9_655 . ?
O4 Mo2 O3 100.7(3) . . ?
O9 Mo2 O3 87.1(3) 9_655 . ?
O9 Mo2 O3 88.5(4) . . ?
O4 Mo2 O3 100.7(3) . 5_565 ?
O9 Mo2 O3 88.5(4) 9_655 5_565 ?
O9 Mo2 O3 87.1(3) . 5_565 ?
O3 Mo2 O3 158.5(5) . 5_565 ?
O4 Mo2 O6 159.0(3) . . ?
O9 Mo2 O6 64.0(4) 9_655 . ?
O9 Mo2 O6 93.5(4) . . ?
O3 Mo2 O6 64.9(4) . . ?
O3 Mo2 O6 94.4(4) 5_565 . ?
O4 Mo2 O6 159.0(3) . 8_565 ?
O9 Mo2 O6 93.5(4) 9_655 8_565 ?
O9 Mo2 O6 64.0(4) . 8_565 ?
O3 Mo2 O6 94.4(4) . 8_565 ?
O3 Mo2 O6 64.9(4) 5_565 8_565 ?
O6 Mo2 O6 42.0(6) . 8_565 ?
O5 P1 O5 180.0 7_775 . ?
O5 P1 O6 109.3(5) 7_775 9_655 ?
O5 P1 O6 70.7(5) . 9_655 ?
O5 P1 O6 109.3(5) 7_775 7_775 ?
O5 P1 O6 70.7(5) . 7_775 ?
O6 P1 O6 109.6(5) 9_655 7_775 ?
O5 P1 O6 70.7(5) 7_775 2_765 ?
O5 P1 O6 109.3(5) . 2_765 ?
O6 P1 O6 70.4(5) 9_655 2_765 ?
O6 P1 O6 70.4(5) 7_775 2_765 ?
O5 P1 O6 109.3(5) 7_775 8_565 ?
O5 P1 O6 70.7(5) . 8_565 ?
O6 P1 O6 109.6(5) 9_655 8_565 ?
O6 P1 O6 109.6(5) 7_775 8_565 ?
O6 P1 O6 180.0 2_765 8_565 ?
O5 P1 O6 70.7(5) 7_775 3_675 ?
O5 P1 O6 109.3(5) . 3_675 ?
O6 P1 O6 180.0(10) 9_655 3_675 ?
O6 P1 O6 70.4(5) 7_775 3_675 ?
O6 P1 O6 109.6(5) 2_765 3_675 ?
O6 P1 O6 70.4(5) 8_565 3_675 ?
O5 P1 O6 70.7(5) 7_775 . ?
O5 P1 O6 109.3(5) . . ?
O6 P1 O6 70.4(5) 9_655 . ?
O6 P1 O6 180.0 7_775 . ?
O6 P1 O6 109.6(5) 2_765 . ?
O6 P1 O6 70.4(5) 8_565 . ?
O6 P1 O6 109.6(5) 3_675 . ?
Mo1 O3 Mo2 137.9(4) . . ?
Mo2 O9 Mo2 139.3(6) . 8_565 ?
Mo1 O1 Mo1 138.7(6) 2_765 . ?
P1 O6 O5 54.4(7) . 7_775 ?
P1 O6 O6 54.8(3) . 9_655 ?
O5 O6 O6 89.7(6) 7_775 9_655 ?
P1 O6 O6 54.8(3) . 8_565 ?
O5 O6 O6 89.7(6) 7_775 8_565 ?
O6 O6 O6 90.3(11) 9_655 8_565 ?
P1 O6 Mo2 123.8(4) . 9_655 ?
O5 O6 Mo2 131.3(3) 7_775 9_655 ?
O6 O6 Mo2 69.0(3) 9_655 9_655 ?
O6 O6 Mo2 131.6(10) 8_565 9_655 ?
P1 O6 Mo2 123.8(4) . . ?
O5 O6 Mo2 131.3(3) 7_775 . ?
O6 O6 Mo2 131.6(10) 9_655 . ?
O6 O6 Mo2 69.0(3) 8_565 . ?
Mo2 O6 Mo2 92.3(5) 9_655 . ?
P1 O6 Mo1 123.5(7) . . ?
O5 O6 Mo1 69.1(7) 7_775 . ?
O6 O6 Mo1 131.1(8) 9_655 . ?
O6 O6 Mo1 131.1(8) 8_565 . ?
Mo2 O6 Mo1 92.2(4) 9_655 . ?
Mo2 O6 Mo1 92.2(4) . . ?
P1 O5 O6 55.0(7) . 7_775 ?
P1 O5 O6 55.0(7) . 9_655 ?
O6 O5 O6 90.3(10) 7_775 9_655 ?
P1 O5 O6 55.0(7) . 8_565 ?
O6 O5 O6 90.3(10) 7_775 8_565 ?
O6 O5 O6 90.3(10) 9_655 8_565 ?
P1 O5 Mo1 124.0(4) . 8_565 ?
O6 O5 Mo1 131.34(13) 7_775 8_565 ?
O6 O5 Mo1 131.34(13) 9_655 8_565 ?
O6 O5 Mo1 69.1(5) 8_565 8_565 ?
P1 O5 Mo1 124.0(4) . 9_655 ?
O6 O5 Mo1 131.34(13) 7_775 9_655 ?
O6 O5 Mo1 69.1(5) 9_655 9_655 ?
O6 O5 Mo1 131.34(13) 8_565 9_655 ?
Mo1 O5 Mo1 91.7(6) 8_565 9_655 ?
P1 O5 Mo1 124.0(4) . 7_775 ?
O6 O5 Mo1 69.1(5) 7_775 7_775 ?
O6 O5 Mo1 131.34(13) 9_655 7_775 ?
O6 O5 Mo1 131.34(13) 8_565 7_775 ?
Mo1 O5 Mo1 91.7(6) 8_565 7_775 ?
Mo1 O5 Mo1 91.7(6) 9_655 7_775 ?
N1 Ag1 N2 117.5(8) . 11_665 ?
N3 Ag2 N3 166.5(8) 6_656 . ?
C1 N1 C2 107.3(18) . . ?
C1 N1 Ag1 131.3(15) . . ?
C2 N1 Ag1 119.9(14) . . ?
C1 N2 N3 107.4(17) . . ?
C1 N2 Ag1 128.9(13) . 12_665 ?
N3 N2 Ag1 123.4(14) . 12_665 ?
N2 N3 C2 105.4(18) . . ?
N2 N3 Ag2 110.4(13) . . ?
C2 N3 Ag2 143.3(14) . . ?
N1 C1 N2 112.7(17) . . ?
N1 C1 H1 123.6 . . ?
N2 C1 H1 123.6 . . ?
N1 C2 N3 107.0(18) . . ?
N1 C2 H2 126.5 . . ?
N3 C2 H2 126.5 . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 Mo1 O3 Mo2 -157.0(6) . . . . ?
O1 Mo1 O3 Mo2 19.4(14) . . . . ?
O1 Mo1 O3 Mo2 101.0(7) 3_675 . . . ?
O3 Mo1 O3 Mo2 -57.2(8) 10 . . . ?
O6 Mo1 O3 Mo2 6.3(6) . . . . ?
O5 Mo1 O3 Mo2 36.8(7) 7_775 . . . ?
O4 Mo2 O3 Mo1 157.6(6) . . . . ?
O9 Mo2 O3 Mo1 56.2(7) 9_655 . . . ?
O9 Mo2 O3 Mo1 -100.8(7) . . . . ?
O3 Mo2 O3 Mo1 -22.5(6) 5_565 . . . ?
O6 Mo2 O3 Mo1 -6.3(6) . . . . ?
O6 Mo2 O3 Mo1 -37.1(7) 8_565 . . . ?
O4 Mo2 O9 Mo2 -155.5(8) . . . 8_565 ?
O9 Mo2 O9 Mo2 24.5(8) 9_655 . . 8_565 ?
O3 Mo2 O9 Mo2 103.9(9) . . . 8_565 ?
O3 Mo2 O9 Mo2 -55.1(9) 5_565 . . 8_565 ?
O6 Mo2 O9 Mo2 39.1(10) . . . 8_565 ?
O6 Mo2 O9 Mo2 8.2(8) 8_565 . . 8_565 ?
O2 Mo1 O1 Mo1 -154.5(9) . . . 2_765 ?
O1 Mo1 O1 Mo1 -52.4(12) 3_675 . . 2_765 ?
O3 Mo1 O1 Mo1 29.0(17) . . . 2_765 ?
O3 Mo1 O1 Mo1 105.4(10) 10 . . 2_765 ?
O6 Mo1 O1 Mo1 40.9(10) . . . 2_765 ?
O5 Mo1 O1 Mo1 9.7(9) 7_775 . . 2_765 ?
O5 P1 O6 O5 180.000(3) . . . 7_775 ?
O6 P1 O6 O5 119.8(6) 9_655 . . 7_775 ?
O6 P1 O6 O5 60.2(6) 2_765 . . 7_775 ?
O6 P1 O6 O5 -119.8(6) 8_565 . . 7_775 ?
O6 P1 O6 O5 -60.2(6) 3_675 . . 7_775 ?
O5 P1 O6 O6 -119.8(6) 7_775 . . 9_655 ?
O5 P1 O6 O6 60.2(6) . . . 9_655 ?
O6 P1 O6 O6 -59.7(12) 2_765 . . 9_655 ?
O6 P1 O6 O6 120.3(12) 8_565 . . 9_655 ?
O6 P1 O6 O6 180.000(2) 3_675 . . 9_655 ?
O5 P1 O6 O6 119.8(6) 7_775 . . 8_565 ?
O5 P1 O6 O6 -60.2(6) . . . 8_565 ?
O6 P1 O6 O6 -120.3(12) 9_655 . . 8_565 ?
O6 P1 O6 O6 180.000(0) 2_765 . . 8_565 ?
O6 P1 O6 O6 59.7(12) 3_675 . . 8_565 ?
O5 P1 O6 Mo2 -119.8(6) 7_775 . . 9_655 ?
O5 P1 O6 Mo2 60.2(6) . . . 9_655 ?
O6 P1 O6 Mo2 -0.001(1) 9_655 . . 9_655 ?
O6 P1 O6 Mo2 -59.7(12) 2_765 . . 9_655 ?
O6 P1 O6 Mo2 120.3(12) 8_565 . . 9_655 ?
O6 P1 O6 Mo2 179.999(1) 3_675 . . 9_655 ?
O5 P1 O6 Mo2 119.8(6) 7_775 . . . ?
O5 P1 O6 Mo2 -60.2(6) . . . . ?
O6 P1 O6 Mo2 -120.3(12) 9_655 . . . ?
O6 P1 O6 Mo2 180.000(1) 2_765 . . . ?
O6 P1 O6 Mo2 0.000(0) 8_565 . . . ?
O6 P1 O6 Mo2 59.7(12) 3_675 . . . ?
O5 P1 O6 Mo1 0.000(1) 7_775 . . . ?
O5 P1 O6 Mo1 180.000(1) . . . . ?
O6 P1 O6 Mo1 119.8(6) 9_655 . . . ?
O6 P1 O6 Mo1 60.2(6) 2_765 . . . ?
O6 P1 O6 Mo1 -119.8(6) 8_565 . . . ?
O6 P1 O6 Mo1 -60.2(6) 3_675 . . . ?
O6 P1 O5 O6 -120.000(2) 9_655 . . 7_775 ?
O6 P1 O5 O6 -60.000(2) 2_765 . . 7_775 ?
O6 P1 O5 O6 120.000(2) 8_565 . . 7_775 ?
O6 P1 O5 O6 60.000(2) 3_675 . . 7_775 ?
O6 P1 O5 O6 180.000(3) . . . 7_775 ?
O6 P1 O5 O6 120.000(3) 7_775 . . 9_655 ?
O6 P1 O5 O6 60.000(4) 2_765 . . 9_655 ?
O6 P1 O5 O6 -120.000(4) 8_565 . . 9_655 ?
O6 P1 O5 O6 180.000(4) 3_675 . . 9_655 ?
O6 P1 O5 O6 -60.000(3) . . . 9_655 ?
O6 P1 O5 O6 120.000(2) 9_655 . . 8_565 ?
O6 P1 O5 O6 -120.000(3) 7_775 . . 8_565 ?
O6 P1 O5 O6 180.000(2) 2_765 . . 8_565 ?
O6 P1 O5 O6 -60.000(2) 3_675 . . 8_565 ?
O6 P1 O5 O6 60.000(3) . . . 8_565 ?
O6 P1 O5 Mo1 120.000(2) 9_655 . . 8_565 ?
O6 P1 O5 Mo1 -120.000(0) 7_775 . . 8_565 ?
O6 P1 O5 Mo1 180.000(1) 2_765 . . 8_565 ?
O6 P1 O5 Mo1 0.000(1) 8_565 . . 8_565 ?
O6 P1 O5 Mo1 -60.000(2) 3_675 . . 8_565 ?
O6 P1 O5 Mo1 60.000(0) . . . 8_565 ?
O6 P1 O5 Mo1 0.000(2) 9_655 . . 9_655 ?
O6 P1 O5 Mo1 120.000(3) 7_775 . . 9_655 ?
O6 P1 O5 Mo1 60.000(3) 2_765 . . 9_655 ?
O6 P1 O5 Mo1 -120.000(3) 8_565 . . 9_655 ?
O6 P1 O5 Mo1 180.000(2) 3_675 . . 9_655 ?
O6 P1 O5 Mo1 -60.000(4) . . . 9_655 ?
O6 P1 O5 Mo1 -120.000(2) 9_655 . . 7_775 ?
O6 P1 O5 Mo1 0.000(0) 7_775 . . 7_775 ?
O6 P1 O5 Mo1 -60.000(1) 2_765 . . 7_775 ?
O6 P1 O5 Mo1 120.000(1) 8_565 . . 7_775 ?
O6 P1 O5 Mo1 60.000(2) 3_675 . . 7_775 ?
O6 P1 O5 Mo1 180.000(0) . . . 7_775 ?
C1 N2 N3 C2 1(3) . . . . ?
Ag1 N2 N3 C2 174.9(15) 12_665 . . . ?
C1 N2 N3 Ag2 -171.2(14) . . . . ?
Ag1 N2 N3 Ag2 3(2) 12_665 . . . ?
C2 N1 C1 N2 -3(2) . . . . ?
Ag1 N1 C1 N2 -169(2) . . . . ?
N3 N2 C1 N1 1(2) . . . . ?
Ag1 N2 C1 N1 -172.5(18) 12_665 . . . ?
C1 N1 C2 N3 3(3) . . . . ?
Ag1 N1 C2 N3 170.9(15) . . . . ?
N2 N3 C2 N1 -2(3) . . . . ?
Ag2 N3 C2 N1 165.0(18) . . . . ?

_refine_diff_density_max         1.085
_refine_diff_density_min         -1.275
_refine_diff_density_rms         0.181

